# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_shelx
_database_code_depnum_ccdc_archive 'CCDC 2208257'
loop_
_audit_author_name
_audit_author_address
'Klaus Wurst'
;University of Innsbruck
Austria
;
_audit_update_record             
;
2022-09-20 deposited with the CCDC.	2022-10-12 downloaded from the CCDC.
;

_audit_creation_date             2022-05-17T12:17:08-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.4.3
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic

#----------------------------------------------------------------------------#
#                   CHEMICAL INFORMATION                                     #
#----------------------------------------------------------------------------#

_chemical_name_systematic        'Lithium oxonitridolithosilicate'
_chemical_formula_moiety         'Li3 Si1  N1  O2'
_chemical_formula_sum            'Li3 Si1  N1  O2'
_chemical_formula_weight         94.92

#----------------------------------------------------------------------------#
#                   UNIT CELL INFORMATION                                    #
#----------------------------------------------------------------------------#

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'C 2/c'
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_Int_Tables_number      15
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   10.4901(3)
_cell_length_b                   11.0342(3)
_cell_length_c                   5.11860(10)
_cell_angle_alpha                90
_cell_angle_beta                 116.1420(10)
_cell_angle_gamma                90
_cell_volume                     531.87(2)
_cell_formula_units_Z            8
_cell_measurement_temperature    297(2)
_cell_measurement_reflns_used    9944
_cell_measurement_theta_min      5.687
_cell_measurement_theta_max      82.425
_cell_measurement_wavelength     0.71073

#----------------------------------------------------------------------------#
#                   CRYSTAL INFORMATION                                      #
#----------------------------------------------------------------------------#

_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.07
_exptl_crystal_density_diffrn    2.371
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             368
_exptl_transmission_factor_min   0.6916
_exptl_transmission_factor_max   0.7481
_exptl_crystal_colour            white
_exptl_crystal_description       prism

#----------------------------------------------------------------------------#
#                   ABSORPTION CORRECTION                                    #
#----------------------------------------------------------------------------#

_exptl_absorpt_coefficient_mu    0.604
_exptl_absorpt_correction_type   multi-scan
_shelx_estimated_absorpt_T_min   0.889
_shelx_estimated_absorpt_T_max   0.959
_exptl_absorpt_process_details   'Bruker (SADABS-2016/2)'

#----------------------------------------------------------------------------#
#                   DATA COLLECTION                                          #
#----------------------------------------------------------------------------#

_diffrn_ambient_temperature      297(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_measurement_device_type  'Bruker D8 QUEST, PHOTON II'
_diffrn_measurement_method       'ω scans'
_diffrn_detector_area_resol_mean 7.4074
_diffrn_radiation_probe          x-ray
_diffrn_reflns_av_R_equivalents  0.0318
_diffrn_reflns_number            24474
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_theta_min         2.844
_diffrn_reflns_theta_max         40.248
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_full 0.889
_diffrn_measured_fraction_theta_max 0.967
_diffrn_reflns_Laue_measured_fraction_full 0.889
_diffrn_reflns_Laue_measured_fraction_max 0.967
_diffrn_reflns_point_group_measured_fraction_full 0.889
_diffrn_reflns_point_group_measured_fraction_max 0.967
_reflns_number_total             1622
_reflns_number_gt                1579
_reflns_threshold_expression     'I > 2σ(I)'

#----------------------------------------------------------------------------#
#                   COMPUTER PROGRAMS USED                                   #
#----------------------------------------------------------------------------#

_computing_data_collection       'Bruker Instrument Service vV6.2.3'
_computing_cell_refinement       'Bruker SAINT-V 8.37A'
_computing_data_reduction        'Bruker SAINT-V 8.37A'
_computing_structure_solution    'XT, VERSION 2014/5'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    'DIAMOND (Brandenburg & Berndt, 1999)'
_computing_publication_material  'WINGX 2013.3'

#----------------------------------------------------------------------------#
#                   STRUCTURE SOLUTION
#----------------------------------------------------------------------------#


#----------------------------------------------------------------------------#
#                   REFINEMENT INFORMATION                                   #
#----------------------------------------------------------------------------#

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0284P)²+0.2771P] where P=(Fo²+2Fc²)/3'
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_coef       0.055(10)
_refine_ls_number_reflns         1622
_refine_ls_number_parameters     66
_refine_ls_number_restraints     0
_refine_ls_number_constraints    0
_refine_ls_R_factor_all          0.0226
_refine_ls_R_factor_gt           0.0222
_refine_ls_wR_factor_ref         0.0594
_refine_ls_wR_factor_gt          0.0591
_refine_ls_goodness_of_fit_ref   1.147
_refine_ls_restrained_S_all      1.147
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0
_refine_diff_density_max         0.516
_refine_diff_density_min         -0.64
_refine_diff_density_rms         0.07

#----------------------------------------------------------------------------#
#                   ATOMIC TYPES, COORDINATES AND THERMAL PARAMETERS         #
#----------------------------------------------------------------------------#

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.006 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_disorder_assembly
_atom_site_disorder_group
Si1 Si 0.22086(2) 0.43007(2) 0.25806(3) 0.00621(6) Uani 1 d . .
O1 O 0.12887(4) 0.31224(3) 0.05472(8) 0.00791(8) Uani 1 d . .
O2 O 0.38906(4) 0.39292(5) 0.37602(10) 0.01470(9) Uani 1 d . .
N1 N 0.17022(5) 0.44522(4) 0.53242(10) 0.00872(8) Uani 1 d . .
Li5 Li 0.27694(16) 0.19757(14) 0.2176(3) 0.0198(3) Uani 1 d . .
Li1 Li 0.5 0.29775(14) 0.25 0.0101(2) Uani 1 d . .
Li2 Li 0.5 0.47456(18) 0.75 0.0153(3) Uani 1 d . .
Li3 Li 0 0.43379(17) -0.25 0.0205(4) Uani 1 d . .
Li4 Li 0 0.3190(3) 0.25 0.0188(4) Uiso 0.76 d . .
Li4A Li 0 0.2747(10) 0.25 0.0189(14) Uiso 0.24 d . .



#----------------------------------------------------------------------------#
#                   MOLECULAR GEOMETRY                                       #
#----------------------------------------------------------------------------#

_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Si1 O2 1.6453(4) . ?
Si1 O1 1.6792(4) . ?
Si1 N1 1.7146(5) . ?
Si1 N1 1.7231(5) 6_565 ?
Si1 Li4 2.6050(16) . ?
Si1 Li3 2.61211(16) . ?
Si1 Li5 2.6604(16) . ?
Si1 Li3 2.7463(10) 5_565 ?
Si1 Li5 2.8215(15) 7 ?
Si1 Li4A 2.868(6) . ?
Si1 Li2 2.9425(4) . ?
Si1 Li5 2.9539(16) 4 ?
O1 Li5 1.8888(14) . ?
O1 Li1 1.9686(11) 7 ?
O1 Li4 2.0058(4) . ?
O1 Li5 2.0358(14) 7 ?
O1 Li4A 2.047(2) . ?
O1 Li3 2.0497(13) . ?
O2 Li1 1.8800(10) . ?
O2 Li2 1.9665(10) . ?
O2 Li2 2.1378(14) 5_666 ?
O2 Li5 2.4180(18) . ?
O2 Li4A 2.544(8) 7_556 ?
N1 Si1 1.7231(5) 6_566 ?
N1 Li5 1.9498(14) 7_556 ?
N1 Li3 2.1876(12) 5_565 ?
N1 Li4 2.223(2) . ?
N1 Li3 2.4894(5) 1_556 ?
N1 Li4A 2.558(8) . ?
Li5 N1 1.9498(14) 7_556 ?
Li5 O1 2.0358(14) 7 ?
Li5 Li5 2.348(3) 7 ?
Li5 Li1 2.5264(17) . ?
Li5 Li3 2.6947(16) 7 ?
Li5 Li4 2.7048(15) 7_556 ?
Li5 Li4A 2.716(2) 7_556 ?
Li5 Si1 2.8216(15) 7 ?
Li5 Li1 2.8362(15) 7 ?
Li1 O2 1.8800(10) 2_655 ?
Li1 O1 1.9686(11) 7 ?
Li1 O1 1.9686(11) 8_556 ?
Li1 Li2 2.512(2) 5_666 ?
Li1 Li5 2.5265(17) 2_655 ?
Li1 Li3 2.555(2) 7 ?
Li1 Li4A 2.681(3) 7 ?
Li1 Li4A 2.681(3) 7_556 ?
Li1 Li5 2.8362(15) 8_556 ?
Li1 Li5 2.8362(15) 7 ?
Li2 O2 1.9665(10) 2_656 ?
Li2 O2 2.1378(14) 5_666 ?
Li2 O2 2.1378(14) 6_566 ?
Li2 Li1 2.512(2) 5_666 ?
Li2 Li2 2.6201(8) 5_667 ?
Li2 Li2 2.6201(8) 5_666 ?
Li2 Li4A 2.750(11) 7_556 ?
Li2 Si1 2.9425(4) 2_656 ?
Li2 Si1 3.1289(7) 5_666 ?
Li2 Si1 3.1289(7) 6_566 ?
Li3 O1 2.0497(13) 2_554 ?
Li3 N1 2.1876(12) 6_565 ?
Li3 N1 2.1876(12) 5_565 ?
Li3 N1 2.4894(5) 2 ?
Li3 N1 2.4894(5) 1_554 ?
Li3 Li1 2.555(2) 7 ?
Li3 Si1 2.61211(16) 2_554 ?
Li3 Li5 2.6947(16) 8_455 ?
Li3 Li5 2.6947(16) 7 ?
Li3 Li4 2.727(4) 5_565 ?
Li4 O1 2.0058(4) 2 ?
Li4 N1 2.223(2) 2 ?
Li4 Si1 2.6050(16) 2 ?
Li4 Li5 2.7048(15) 8_455 ?
Li4 Li5 2.7048(15) 7_556 ?
Li4 Li3 2.727(4) 5_565 ?
Li4 Li3 2.8554(17) 1_556 ?
Li4 Li1 2.8655(16) 7 ?
Li4A O1 2.047(2) 2 ?
Li4A O2 2.544(8) 8_455 ?
Li4A O2 2.544(8) 7_556 ?
Li4A N1 2.558(8) 2 ?
Li4A Li1 2.681(3) 7 ?
Li4A Li1 2.681(3) 7_556 ?
Li4A Li5 2.716(2) 7_556 ?
Li4A Li5 2.716(2) 8_455 ?
Li4A Li2 2.750(11) 7_556 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Si1 O1 105.37(2) . . ?
O2 Si1 N1 113.13(2) . . ?
O1 Si1 N1 106.40(2) . . ?
O2 Si1 N1 114.15(3) . 6_565 ?
O1 Si1 N1 106.24(2) . 6_565 ?
N1 Si1 N1 110.841(19) . 6_565 ?
O2 Si1 Li4 133.72(6) . . ?
O1 Si1 Li4 50.35(5) . . ?
N1 Si1 Li4 57.62(4) . . ?
N1 Si1 Li4 110.83(5) 6_565 . ?
O2 Si1 Li3 134.96(2) . . ?
O1 Si1 Li3 51.66(4) . . ?
N1 Si1 Li3 110.786(18) . . ?
N1 Si1 Li3 56.21(4) 6_565 . ?
Li4 Si1 Li3 66.36(3) . . ?
O2 Si1 Li5 63.27(4) . . ?
O1 Si1 Li5 44.89(4) . . ?
N1 Si1 Li5 108.47(3) . . ?
N1 Si1 Li5 137.00(3) 6_565 . ?
Li4 Si1 Li5 76.76(7) . . ?
Li3 Si1 Li5 93.86(5) . . ?
O2 Si1 Li3 154.56(3) . 5_565 ?
O1 Si1 Li3 99.41(3) . 5_565 ?
N1 Si1 Li3 52.78(2) . 5_565 ?
N1 Si1 Li3 62.88(3) 6_565 5_565 ?
Li4 Si1 Li3 61.21(8) . 5_565 ?
Li3 Si1 Li3 66.68(3) . 5_565 ?
Li5 Si1 Li3 137.76(5) . 5_565 ?
O2 Si1 Li5 77.13(3) . 7 ?
O1 Si1 Li5 45.55(3) . 7 ?
N1 Si1 Li5 151.49(4) . 7 ?
N1 Si1 Li5 86.42(3) 6_565 7 ?
Li4 Si1 Li5 95.57(5) . 7 ?
Li3 Si1 Li5 59.31(4) . 7 ?
Li5 Si1 Li5 50.61(5) . 7 ?
Li3 Si1 Li5 125.99(3) 5_565 7 ?
O2 Si1 Li4A 125.82(16) . . ?
O1 Si1 Li4A 44.62(11) . . ?
N1 Si1 Li4A 61.98(9) . . ?
N1 Si1 Li4A 117.34(13) 6_565 . ?
Li4 Si1 Li4A 8.67(15) . . ?
Li3 Si1 Li4A 68.81(6) . . ?
Li5 Si1 Li4A 68.11(17) . . ?
Li3 Si1 Li4A 69.88(18) 5_565 . ?
Li5 Si1 Li4A 90.16(11) 7 . ?
O2 Si1 Li2 39.25(3) . . ?
O1 Si1 Li2 137.99(4) . . ?
N1 Si1 Li2 80.412(18) . . ?
N1 Si1 Li2 109.70(4) 6_565 . ?
Li4 Si1 Li2 129.40(2) . . ?
Li3 Si1 Li2 163.96(4) . . ?
Li5 Si1 Li2 93.25(5) . . ?
Li3 Si1 Li2 115.88(3) 5_565 . ?
Li5 Si1 Li2 116.00(4) 7 . ?
Li4A Si1 Li2 127.23(6) . . ?
O2 Si1 Li5 104.26(3) . 4 ?
O1 Si1 Li5 142.32(3) . 4 ?
N1 Si1 Li5 82.38(3) . 4 ?
N1 Si1 Li5 39.16(3) 6_565 4 ?
Li4 Si1 Li5 117.45(7) . 4 ?
Li3 Si1 Li5 90.76(5) . 4 ?
Li5 Si1 Li5 165.687(12) . 4 ?
Li3 Si1 Li5 56.28(4) 5_565 4 ?
Li5 Si1 Li5 122.16(5) 7 4 ?
Li4A Si1 Li5 126.11(17) . 4 ?
Li2 Si1 Li5 79.10(5) . 4 ?
Si1 O1 Li5 96.25(6) . . ?
Si1 O1 Li1 167.14(4) . 7 ?
Li5 O1 Li1 94.64(6) . 7 ?
Si1 O1 Li4 89.52(8) . . ?
Li5 O1 Li4 114.13(8) . . ?
Li1 O1 Li4 92.27(6) 7 . ?
Si1 O1 Li5 98.38(5) . 7 ?
Li5 O1 Li5 73.37(6) . 7 ?
Li1 O1 Li5 78.22(5) 7 7 ?
Li4 O1 Li5 168.58(5) . 7 ?
Si1 O1 Li4A 100.2(2) . . ?
Li5 O1 Li4A 103.9(2) . . ?
Li1 O1 Li4A 83.76(18) 7 . ?
Li4 O1 Li4A 13.8(3) . . ?
Li5 O1 Li4A 161.4(2) 7 . ?
Si1 O1 Li3 88.35(4) . . ?
Li5 O1 Li3 155.87(5) . . ?
Li1 O1 Li3 78.93(6) 7 . ?
Li4 O1 Li3 89.50(7) . . ?
Li5 O1 Li3 82.54(4) 7 . ?
Li4A O1 Li3 98.52(19) . . ?
Si1 O2 Li1 137.65(3) . . ?
Si1 O2 Li2 108.79(3) . . ?
Li1 O2 Li2 113.55(3) . . ?
Si1 O2 Li2 110.93(4) . 5_666 ?
Li1 O2 Li2 77.11(6) . 5_666 ?
Li2 O2 Li2 79.22(2) . 5_666 ?
Si1 O2 Li5 79.31(4) . . ?
Li1 O2 Li5 70.74(5) . . ?
Li2 O2 Li5 136.60(6) . . ?
Li2 O2 Li5 139.25(5) 5_666 . ?
Si1 O2 Li4A 121.21(5) . 7_556 ?
Li1 O2 Li4A 72.85(9) . 7_556 ?
Li2 O2 Li4A 73.87(17) . 7_556 ?
Li2 O2 Li4A 126.49(8) 5_666 7_556 ?
Li5 O2 Li4A 66.31(16) . 7_556 ?
Si1 N1 Si1 120.77(3) . 6_566 ?
Si1 N1 Li5 110.95(5) . 7_556 ?
Si1 N1 Li5 106.91(6) 6_566 7_556 ?
Si1 N1 Li3 88.60(2) . 5_565 ?
Si1 N1 Li3 82.90(4) 6_566 5_565 ?
Li5 N1 Li3 147.14(6) 7_556 5_565 ?
Si1 N1 Li4 81.736(19) . . ?
Si1 N1 Li4 149.11(5) 6_566 . ?
Li5 N1 Li4 80.52(8) 7_556 . ?
Li3 N1 Li4 76.38(8) 5_565 . ?
Si1 N1 Li3 154.64(3) . 1_556 ?
Si1 N1 Li3 79.09(4) 6_566 1_556 ?
Li5 N1 Li3 73.62(6) 7_556 1_556 ?
Li3 N1 Li3 77.82(4) 5_565 1_556 ?
Li4 N1 Li3 74.35(3) . 1_556 ?
Si1 N1 Li4A 81.745(18) . . ?
Si1 N1 Li4A 153.96(8) 6_566 . ?
Li5 N1 Li4A 72.67(16) 7_556 . ?
Li3 N1 Li4A 84.97(17) 5_565 . ?
Li4 N1 Li4A 8.58(14) . . ?
Li3 N1 Li4A 75.87(5) 1_556 . ?
O1 Li5 N1 140.51(8) . 7_556 ?
O1 Li5 O1 106.63(6) . 7 ?
N1 Li5 O1 108.84(7) 7_556 7 ?
O1 Li5 Li5 56.19(5) . 7 ?
N1 Li5 Li5 154.28(12) 7_556 7 ?
O1 Li5 Li5 50.44(5) 7 7 ?
O1 Li5 O2 74.62(6) . . ?
N1 Li5 O2 123.00(8) 7_556 . ?
O1 Li5 O2 88.05(6) 7 . ?
Li5 Li5 O2 75.94(8) 7 . ?
O1 Li5 Li1 107.07(7) . . ?
N1 Li5 Li1 108.86(7) 7_556 . ?
O1 Li5 Li1 49.71(4) 7 . ?
Li5 Li5 Li1 71.06(7) 7 . ?
O2 Li5 Li1 44.63(4) . . ?
O1 Li5 Si1 38.86(3) . . ?
N1 Li5 Si1 137.46(7) 7_556 . ?
O1 Li5 Si1 107.17(6) 7 . ?
Li5 Li5 Si1 68.25(7) 7 . ?
O2 Li5 Si1 37.42(3) . . ?
Li1 Li5 Si1 78.64(6) . . ?
O1 Li5 Li3 155.56(7) . 7 ?
N1 Li5 Li3 62.41(5) 7_556 7 ?
O1 Li5 Li3 48.95(3) 7 7 ?
Li5 Li5 Li3 99.38(8) 7 7 ?
O2 Li5 Li3 100.25(6) . 7 ?
Li1 Li5 Li3 58.49(6) . 7 ?
Si1 Li5 Li3 136.86(7) . 7 ?
O1 Li5 Li4 131.93(10) . 7_556 ?
N1 Li5 Li4 54.16(8) 7_556 7_556 ?
O1 Li5 Li4 102.76(6) 7 7_556 ?
Li5 Li5 Li4 136.81(12) 7 7_556 ?
O2 Li5 Li4 69.24(8) . 7_556 ?
Li1 Li5 Li4 66.33(5) . 7_556 ?
Si1 Li5 Li4 96.30(9) . 7_556 ?
Li3 Li5 Li4 63.85(5) 7 7_556 ?
O1 Li5 Li4A 123.0(2) . 7_556 ?
N1 Li5 Li4A 64.1(2) 7_556 7_556 ?
O1 Li5 Li4A 103.27(6) 7 7_556 ?
Li5 Li5 Li4A 129.6(2) 7 7_556 ?
O2 Li5 Li4A 59.1(2) . 7_556 ?
Li1 Li5 Li4A 61.39(11) . 7_556 ?
Si1 Li5 Li4A 86.3(2) . 7_556 ?
Li3 Li5 Li4A 70.01(14) 7 7_556 ?
Li4 Li5 Li4A 10.4(2) 7_556 7_556 ?
O1 Li5 Si1 105.74(6) . 7 ?
N1 Li5 Si1 93.15(6) 7_556 7 ?
O1 Li5 Si1 36.07(3) 7 7 ?
Li5 Li5 Si1 61.14(7) 7 7 ?
O2 Li5 Si1 123.14(5) . 7 ?
Li1 Li5 Si1 85.16(4) . 7 ?
Si1 Li5 Si1 129.39(5) . 7 ?
Li3 Li5 Si1 56.47(3) 7 7 ?
Li4 Li5 Si1 120.21(6) 7_556 7 ?
Li4A Li5 Si1 126.24(13) 7_556 7 ?
O1 Li5 Li1 43.77(5) . 7 ?
N1 Li5 Li1 117.25(8) 7_556 7 ?
O1 Li5 Li1 92.80(5) 7 7 ?
Li5 Li5 Li1 57.41(7) 7 7 ?
O2 Li5 Li1 115.65(6) . 7 ?
Li1 Li5 Li1 128.47(5) . 7 ?
Si1 Li5 Li1 82.46(5) . 7 ?
Li3 Li5 Li1 126.91(7) 7 7 ?
Li4 Li5 Li1 163.99(6) 7_556 7 ?
Li4A Li5 Li1 162.56(11) 7_556 7 ?
Si1 Li5 Li1 71.07(4) 7 7 ?
O2 Li1 O2 112.09(9) 2_655 . ?
O2 Li1 O1 112.66(2) 2_655 7 ?
O2 Li1 O1 107.659(19) . 7 ?
O2 Li1 O1 107.659(18) 2_655 8_556 ?
O2 Li1 O1 112.66(2) . 8_556 ?
O1 Li1 O1 103.87(8) 7 8_556 ?
O2 Li1 Li2 56.05(4) 2_655 5_666 ?
O2 Li1 Li2 56.05(4) . 5_666 ?
O1 Li1 Li2 128.06(4) 7 5_666 ?
O1 Li1 Li2 128.06(4) 8_556 5_666 ?
O2 Li1 Li5 156.53(4) 2_655 . ?
O2 Li1 Li5 64.63(4) . . ?
O1 Li1 Li5 52.07(4) 7 . ?
O1 Li1 Li5 94.31(6) 8_556 . ?
Li2 Li1 Li5 115.95(4) 5_666 . ?
O2 Li1 Li5 64.63(4) 2_655 2_655 ?
O2 Li1 Li5 156.53(4) . 2_655 ?
O1 Li1 Li5 94.31(6) 7 2_655 ?
O1 Li1 Li5 52.07(4) 8_556 2_655 ?
Li2 Li1 Li5 115.95(4) 5_666 2_655 ?
Li5 Li1 Li5 128.10(9) . 2_655 ?
O2 Li1 Li3 123.95(4) 2_655 7 ?
O2 Li1 Li3 123.95(4) . 7 ?
O1 Li1 Li3 51.94(4) 7 7 ?
O1 Li1 Li3 51.94(4) 8_556 7 ?
Li2 Li1 Li3 180 5_666 7 ?
Li5 Li1 Li3 64.05(4) . 7 ?
Li5 Li1 Li3 64.05(4) 2_655 7 ?
O2 Li1 Li4A 65.07(17) 2_655 7 ?
O2 Li1 Li4A 138.96(12) . 7 ?
O1 Li1 Li4A 49.37(13) 7 7 ?
O1 Li1 Li4A 106.48(17) 8_556 7 ?
Li2 Li1 Li4A 107.3(2) 5_666 7 ?
Li5 Li1 Li4A 101.33(12) . 7 ?
Li5 Li1 Li4A 62.79(9) 2_655 7 ?
Li3 Li1 Li4A 72.7(2) 7 7 ?
O2 Li1 Li4A 138.96(12) 2_655 7_556 ?
O2 Li1 Li4A 65.07(17) . 7_556 ?
O1 Li1 Li4A 106.48(17) 7 7_556 ?
O1 Li1 Li4A 49.37(13) 8_556 7_556 ?
Li2 Li1 Li4A 107.3(2) 5_666 7_556 ?
Li5 Li1 Li4A 62.79(9) . 7_556 ?
Li5 Li1 Li4A 101.33(12) 2_655 7_556 ?
Li3 Li1 Li4A 72.7(2) 7 7_556 ?
Li4A Li1 Li4A 145.3(4) 7 7_556 ?
O2 Li1 Li5 73.78(3) 2_655 8_556 ?
O2 Li1 Li5 105.01(4) . 8_556 ?
O1 Li1 Li5 140.39(7) 7 8_556 ?
O1 Li1 Li5 41.59(3) 8_556 8_556 ?
Li2 Li1 Li5 88.96(5) 5_666 8_556 ?
Li5 Li1 Li5 129.65(6) . 8_556 ?
Li5 Li1 Li5 51.53(5) 2_655 8_556 ?
Li3 Li1 Li5 91.04(5) 7 8_556 ?
Li4A Li1 Li5 112.35(4) 7 8_556 ?
Li4A Li1 Li5 68.33(4) 7_556 8_556 ?
O2 Li1 Li5 105.01(4) 2_655 7 ?
O2 Li1 Li5 73.78(3) . 7 ?
O1 Li1 Li5 41.59(3) 7 7 ?
O1 Li1 Li5 140.39(7) 8_556 7 ?
Li2 Li1 Li5 88.96(5) 5_666 7 ?
Li5 Li1 Li5 51.53(5) . 7 ?
Li5 Li1 Li5 129.65(6) 2_655 7 ?
Li3 Li1 Li5 91.04(5) 7 7 ?
Li4A Li1 Li5 68.33(4) 7 7 ?
Li4A Li1 Li5 112.35(4) 7_556 7 ?
Li5 Li1 Li5 177.91(9) 8_556 7 ?
O2 Li2 O2 125.47(11) . 2_656 ?
O2 Li2 O2 100.78(2) . 5_666 ?
O2 Li2 O2 116.09(3) 2_656 5_666 ?
O2 Li2 O2 116.09(3) . 6_566 ?
O2 Li2 O2 100.78(2) 2_656 6_566 ?
O2 Li2 O2 93.68(8) 5_666 6_566 ?
O2 Li2 Li1 117.27(5) . 5_666 ?
O2 Li2 Li1 117.27(5) 2_656 5_666 ?
O2 Li2 Li1 46.84(4) 5_666 5_666 ?
O2 Li2 Li1 46.84(4) 6_566 5_666 ?
O2 Li2 Li2 142.59(6) . 5_667 ?
O2 Li2 Li2 53.28(3) 2_656 5_667 ?
O2 Li2 Li2 112.49(10) 5_666 5_667 ?
O2 Li2 Li2 47.50(5) 6_566 5_667 ?
Li1 Li2 Li2 77.63(8) 5_666 5_667 ?
O2 Li2 Li2 53.28(3) . 5_666 ?
O2 Li2 Li2 142.59(6) 2_656 5_666 ?
O2 Li2 Li2 47.50(5) 5_666 5_666 ?
O2 Li2 Li2 112.49(10) 6_566 5_666 ?
Li1 Li2 Li2 77.63(8) 5_666 5_666 ?
Li2 Li2 Li2 155.26(17) 5_667 5_666 ?
O2 Li2 Li4A 62.73(5) . 7_556 ?
O2 Li2 Li4A 62.73(5) 2_656 7_556 ?
O2 Li2 Li4A 133.16(4) 5_666 7_556 ?
O2 Li2 Li4A 133.16(4) 6_566 7_556 ?
Li1 Li2 Li4A 180 5_666 7_556 ?
Li2 Li2 Li4A 102.37(8) 5_667 7_556 ?
Li2 Li2 Li4A 102.37(8) 5_666 7_556 ?
O2 Li2 Si1 134.07(7) . 2_656 ?
O2 Li2 Si1 31.961(13) 2_656 2_656 ?
O2 Li2 Si1 84.467(19) 5_666 2_656 ?
O2 Li2 Si1 108.95(3) 6_566 2_656 ?
Li1 Li2 Si1 99.60(4) 5_666 2_656 ?
Li2 Li2 Si1 68.169(12) 5_667 2_656 ?
Li2 Li2 Si1 116.318(4) 5_666 2_656 ?
Li4A Li2 Si1 80.40(4) 7_556 2_656 ?
O2 Li2 Si1 31.960(13) . . ?
O2 Li2 Si1 134.07(7) 2_656 . ?
O2 Li2 Si1 108.95(3) 5_666 . ?
O2 Li2 Si1 84.467(19) 6_566 . ?
Li1 Li2 Si1 99.60(4) 5_666 . ?
Li2 Li2 Si1 116.318(3) 5_667 . ?
Li2 Li2 Si1 68.169(12) 5_666 . ?
Li4A Li2 Si1 80.40(4) 7_556 . ?
Si1 Li2 Si1 160.79(7) 2_656 . ?
O2 Li2 Si1 107.287(14) . 5_666 ?
O2 Li2 Si1 90.631(13) 2_656 5_666 ?
O2 Li2 Si1 29.417(12) 5_666 5_666 ?
O2 Li2 Si1 114.26(7) 6_566 5_666 ?
Li1 Li2 Si1 70.35(3) 5_666 5_666 ?
Li2 Li2 Si1 110.09(5) 5_667 5_666 ?
Li2 Li2 Si1 60.81(3) 5_666 5_666 ?
Li4A Li2 Si1 109.65(3) 7_556 5_666 ?
Si1 Li2 Si1 58.881(6) 2_656 5_666 ?
Si1 Li2 Si1 128.980(14) . 5_666 ?
O2 Li2 Si1 90.630(13) . 6_566 ?
O2 Li2 Si1 107.286(14) 2_656 6_566 ?
O2 Li2 Si1 114.26(7) 5_666 6_566 ?
O2 Li2 Si1 29.417(12) 6_566 6_566 ?
Li1 Li2 Si1 70.35(3) 5_666 6_566 ?
Li2 Li2 Si1 60.81(2) 5_667 6_566 ?
Li2 Li2 Si1 110.09(5) 5_666 6_566 ?
Li4A Li2 Si1 109.65(3) 7_556 6_566 ?
Si1 Li2 Si1 128.980(14) 2_656 6_566 ?
Si1 Li2 Si1 58.881(6) . 6_566 ?
Si1 Li2 Si1 140.69(7) 5_666 6_566 ?
O1 Li3 O1 98.26(8) 2_554 . ?
O1 Li3 N1 167.12(3) 2_554 6_565 ?
O1 Li3 N1 79.853(16) . 6_565 ?
O1 Li3 N1 79.851(16) 2_554 5_565 ?
O1 Li3 N1 167.12(3) . 5_565 ?
N1 Li3 N1 104.79(8) 6_565 5_565 ?
O1 Li3 N1 90.63(3) 2_554 2 ?
O1 Li3 N1 93.17(3) . 2 ?
N1 Li3 N1 102.18(4) 6_565 2 ?
N1 Li3 N1 74.17(3) 5_565 2 ?
O1 Li3 N1 93.17(3) 2_554 1_554 ?
O1 Li3 N1 90.63(3) . 1_554 ?
N1 Li3 N1 74.17(3) 6_565 1_554 ?
N1 Li3 N1 102.18(4) 5_565 1_554 ?
N1 Li3 N1 174.19(9) 2 1_554 ?
O1 Li3 Li1 49.13(4) 2_554 7 ?
O1 Li3 Li1 49.13(4) . 7 ?
N1 Li3 Li1 127.61(4) 6_565 7 ?
N1 Li3 Li1 127.61(4) 5_565 7 ?
N1 Li3 Li1 92.90(4) 2 7 ?
N1 Li3 Li1 92.90(4) 1_554 7 ?
O1 Li3 Si1 39.985(11) 2_554 2_554 ?
O1 Li3 Si1 138.21(8) . 2_554 ?
N1 Li3 Si1 140.82(7) 6_565 2_554 ?
N1 Li3 Si1 40.889(13) 5_565 2_554 ?
N1 Li3 Si1 87.121(12) 2 2_554 ?
N1 Li3 Si1 92.971(12) 1_554 2_554 ?
Li1 Li3 Si1 89.10(4) 7 2_554 ?
O1 Li3 Si1 138.21(8) 2_554 . ?
O1 Li3 Si1 39.986(11) . . ?
N1 Li3 Si1 40.889(13) 6_565 . ?
N1 Li3 Si1 140.82(7) 5_565 . ?
N1 Li3 Si1 92.971(12) 2 . ?
N1 Li3 Si1 87.121(12) 1_554 . ?
Li1 Li3 Si1 89.10(4) 7 . ?
Si1 Li3 Si1 178.20(8) 2_554 . ?
O1 Li3 Li5 48.51(4) 2_554 8_455 ?
O1 Li3 Li5 87.63(6) . 8_455 ?
N1 Li3 Li5 143.39(3) 6_565 8_455 ?
N1 Li3 Li5 81.59(4) 5_565 8_455 ?
N1 Li3 Li5 43.96(3) 2 8_455 ?
N1 Li3 Li5 140.74(6) 1_554 8_455 ?
Li1 Li3 Li5 57.46(5) 7 8_455 ?
Si1 Li3 Li5 64.22(4) 2_554 8_455 ?
Si1 Li3 Li5 114.71(5) . 8_455 ?
O1 Li3 Li5 87.63(6) 2_554 7 ?
O1 Li3 Li5 48.51(4) . 7 ?
N1 Li3 Li5 81.59(4) 6_565 7 ?
N1 Li3 Li5 143.39(3) 5_565 7 ?
N1 Li3 Li5 140.74(6) 2 7 ?
N1 Li3 Li5 43.96(3) 1_554 7 ?
Li1 Li3 Li5 57.46(5) 7 7 ?
Si1 Li3 Li5 114.71(5) 2_554 7 ?
Si1 Li3 Li5 64.22(4) . 7 ?
Li5 Li3 Li5 114.92(10) 8_455 7 ?
O1 Li3 Li4 130.87(4) 2_554 5_565 ?
O1 Li3 Li4 130.87(4) . 5_565 ?
N1 Li3 Li4 52.39(4) 6_565 5_565 ?
N1 Li3 Li4 52.39(4) 5_565 5_565 ?
N1 Li3 Li4 87.10(4) 2 5_565 ?
N1 Li3 Li4 87.10(4) 1_554 5_565 ?
Li1 Li3 Li4 180 7 5_565 ?
Si1 Li3 Li4 90.90(4) 2_554 5_565 ?
Si1 Li3 Li4 90.90(4) . 5_565 ?
Li5 Li3 Li4 122.54(5) 8_455 5_565 ?
Li5 Li3 Li4 122.54(5) 7 5_565 ?
O1 Li4 O1 175.71(19) . 2 ?
O1 Li4 N1 102.95(7) . 2 ?
O1 Li4 N1 79.80(5) 2 2 ?
O1 Li4 N1 79.80(5) . . ?
O1 Li4 N1 102.95(7) 2 . ?
N1 Li4 N1 102.45(14) 2 . ?
O1 Li4 Si1 40.14(3) . . ?
O1 Li4 Si1 143.11(11) 2 . ?
N1 Li4 Si1 99.77(10) 2 . ?
N1 Li4 Si1 40.65(3) . . ?
O1 Li4 Si1 143.11(11) . 2 ?
O1 Li4 Si1 40.13(3) 2 2 ?
N1 Li4 Si1 40.64(3) 2 2 ?
N1 Li4 Si1 99.77(10) . 2 ?
Si1 Li4 Si1 123.90(13) . 2 ?
O1 Li4 Li5 88.24(3) . 8_455 ?
O1 Li4 Li5 91.47(3) 2 8_455 ?
N1 Li4 Li5 45.32(4) 2 8_455 ?
N1 Li4 Li5 142.00(13) . 8_455 ?
Si1 Li4 Li5 114.61(5) . 8_455 ?
Si1 Li4 Li5 69.35(4) 2 8_455 ?
O1 Li4 Li5 91.47(3) . 7_556 ?
O1 Li4 Li5 88.24(3) 2 7_556 ?
N1 Li4 Li5 142.00(13) 2 7_556 ?
N1 Li4 Li5 45.32(4) . 7_556 ?
Si1 Li4 Li5 69.35(4) . 7_556 ?
Si1 Li4 Li5 114.61(5) 2 7_556 ?
Li5 Li4 Li5 172.23(16) 8_455 7_556 ?
O1 Li4 Li3 92.15(10) . 5_565 ?
O1 Li4 Li3 92.15(10) 2 5_565 ?
N1 Li4 Li3 51.22(7) 2 5_565 ?
N1 Li4 Li3 51.22(7) . 5_565 ?
Si1 Li4 Li3 61.95(7) . 5_565 ?
Si1 Li4 Li3 61.95(7) 2 5_565 ?
Li5 Li4 Li3 93.89(8) 8_455 5_565 ?
Li5 Li4 Li3 93.89(8) 7_556 5_565 ?
O1 Li4 Li3 45.87(4) . . ?
O1 Li4 Li3 136.84(9) 2 . ?
N1 Li4 Li3 57.09(5) 2 . ?
N1 Li4 Li3 89.31(8) . . ?
Si1 Li4 Li3 56.94(4) . . ?
Si1 Li4 Li3 97.38(8) 2 . ?
Li5 Li4 Li3 57.90(4) 8_455 . ?
Li5 Li4 Li3 126.26(6) 7_556 . ?
Li3 Li4 Li3 63.68(7) 5_565 . ?
O1 Li4 Li3 136.84(9) . 1_556 ?
O1 Li4 Li3 45.87(4) 2 1_556 ?
N1 Li4 Li3 89.31(8) 2 1_556 ?
N1 Li4 Li3 57.09(5) . 1_556 ?
Si1 Li4 Li3 97.38(8) . 1_556 ?
Si1 Li4 Li3 56.94(4) 2 1_556 ?
Li5 Li4 Li3 126.26(6) 8_455 1_556 ?
Li5 Li4 Li3 57.90(4) 7_556 1_556 ?
Li3 Li4 Li3 63.68(7) 5_565 1_556 ?
Li3 Li4 Li3 127.36(13) . 1_556 ?
O1 Li4 Li1 43.35(4) . 7 ?
O1 Li4 Li1 133.91(10) 2 7 ?
N1 Li4 Li1 90.97(2) 2 7 ?
N1 Li4 Li1 123.12(3) . 7 ?
Si1 Li4 Li1 82.857(18) . 7 ?
Si1 Li4 Li1 123.186(9) 2 7 ?
Li5 Li4 Li1 53.85(4) 8_455 7 ?
Li5 Li4 Li1 121.93(7) 7_556 7 ?
Li3 Li4 Li1 116.73(7) 5_565 7 ?
Li3 Li4 Li1 53.05(4) . 7 ?
Li3 Li4 Li1 179.59(12) 1_556 7 ?
O1 Li4A O1 156.6(6) . 2 ?
O1 Li4A O2 87.79(17) . 8_455 ?
O1 Li4A O2 109.5(2) 2 8_455 ?
O1 Li4A O2 109.5(2) . 7_556 ?
O1 Li4A O2 87.79(17) 2 7_556 ?
O2 Li4A O2 86.8(3) 8_455 7_556 ?
O1 Li4A N1 91.2(3) . 2 ?
O1 Li4A N1 71.3(2) 2 2 ?
O2 Li4A N1 97.785(15) 8_455 2 ?
O2 Li4A N1 159.010(19) 7_556 2 ?
O1 Li4A N1 71.3(2) . . ?
O1 Li4A N1 91.2(3) 2 . ?
O2 Li4A N1 159.010(19) 8_455 . ?
O2 Li4A N1 97.786(15) 7_556 . ?
N1 Li4A N1 85.3(3) 2 . ?
O1 Li4A Li1 46.88(6) . 7 ?
O1 Li4A Li1 143.55(8) 2 7 ?
O2 Li4A Li1 42.07(9) 8_455 7 ?
O2 Li4A Li1 108.0(3) 7_556 7 ?
N1 Li4A Li1 88.47(10) 2 7 ?
N1 Li4A Li1 117.71(17) . 7 ?
O1 Li4A Li1 143.55(8) . 7_556 ?
O1 Li4A Li1 46.88(6) 2 7_556 ?
O2 Li4A Li1 108.0(3) 8_455 7_556 ?
O2 Li4A Li1 42.07(9) 7_556 7_556 ?
N1 Li4A Li1 117.71(17) 2 7_556 ?
N1 Li4A Li1 88.47(10) . 7_556 ?
Li1 Li4A Li1 145.3(4) 7 7_556 ?
O1 Li4A Li5 90.27(9) . 7_556 ?
O1 Li4A Li5 87.11(8) 2 7_556 ?
O2 Li4A Li5 138.0(4) 8_455 7_556 ?
O2 Li4A Li5 54.61(7) 7_556 7_556 ?
N1 Li4A Li5 124.2(4) 2 7_556 ?
N1 Li4A Li5 43.26(8) . 7_556 ?
Li1 Li4A Li5 128.98(9) 7 7_556 ?
Li1 Li4A Li5 55.82(4) 7_556 7_556 ?
O1 Li4A Li5 87.11(8) . 8_455 ?
O1 Li4A Li5 90.27(9) 2 8_455 ?
O2 Li4A Li5 54.61(7) 8_455 8_455 ?
O2 Li4A Li5 138.0(4) 7_556 8_455 ?
N1 Li4A Li5 43.26(8) 2 8_455 ?
N1 Li4A Li5 124.2(4) . 8_455 ?
Li1 Li4A Li5 55.82(4) 7 8_455 ?
Li1 Li4A Li5 128.98(9) 7_556 8_455 ?
Li5 Li4A Li5 167.0(5) 7_556 8_455 ?
O1 Li4A Li2 101.7(3) . 7_556 ?
O1 Li4A Li2 101.7(3) 2 7_556 ?
O2 Li4A Li2 43.39(17) 8_455 7_556 ?
O2 Li4A Li2 43.39(17) 7_556 7_556 ?
N1 Li4A Li2 137.36(16) 2 7_556 ?
N1 Li4A Li2 137.36(16) . 7_556 ?
Li1 Li4A Li2 72.7(2) 7 7_556 ?
Li1 Li4A Li2 72.7(2) 7_556 7_556 ?
Li5 Li4A Li2 96.5(2) 7_556 7_556 ?
Li5 Li4A Li2 96.5(2) 8_455 7_556 ?
O1 Li4A Si1 35.19(12) . . ?
O1 Li4A Si1 125.1(4) 2 . ?
O2 Li4A Si1 122.96(5) 8_455 . ?
O2 Li4A Si1 108.96(3) 7_556 . ?
N1 Li4A Si1 85.8(3) 2 . ?
N1 Li4A Si1 36.27(9) . . ?
Li1 Li4A Si1 81.50(7) 7 . ?
Li1 Li4A Si1 120.28(12) 7_556 . ?
Li5 Li4A Si1 65.46(11) 7_556 . ?
Li5 Li4A Si1 106.3(2) 8_455 . ?
Li2 Li4A Si1 126.72(17) 7_556 . ?


# END of CIF
_exptl_crystal_preparation       Luminescent
